1 / 25

300 likes | 567 Vues

EML 4230 Introduction to Composite Materials. Chapter 4 Macromechanical Analysis of a Laminate Laminate Analysis: Example Dr . Autar Kaw Department of Mechanical Engineering University of South Florida, Tampa, FL 33620 Courtesy of the Textbook Mechanics of Composite Materials by Kaw.

Télécharger la présentation
## EML 4230 Introduction to Composite Materials

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**EML 4230 Introduction to Composite Materials**Chapter 4 Macromechanical Analysis of a Laminate Laminate Analysis: Example Dr. Autar Kaw Department of Mechanical Engineering University of South Florida, Tampa, FL 33620 Courtesy of the Textbook Mechanics of Composite Materials by Kaw**Problem**A [0/30/-45] Graphite/Epoxy laminate is subjected to a load of Nx = Ny = 1000 N/m. Use the unidirectional properties from Table 2.1 of Graphite/Epoxy. Assume each lamina has a thickness of 5 mm. Find • the three stiffness matrices [A], [B] and [D] for a three ply [0/30/-45] Graphite/Epoxy laminate. • mid-plane strains and curvatures. • global and local stresses on top surface of 300 ply. • percentage of load Nx taken by each ply.**Solution**A) The reduced stiffness matrix for the OoGraphite/Epoxy ply is**Coordinates of top & bottom of plies**The total thickness of the laminate is h = (0.005)(3) = 0.015 m. h0=-0.0075 m h1=-0.0025 m h2=0.0025 m h3=0.0075 m**B) Since the applied load is Nx =Ny = 1000 N/m, the**mid-plane strains and curvatures can be found by solving the following set of simultaneous linear equations Setting up the 6x6 matrix**Global Strains/Stresses at top of 30o ply**C) The strains and stresses at thetop surface of the 300 ply are found as follows. The top surface of the 300 ply is located at z = h1 = -0.0025 m.**Local Strains/Stresses at top of 30o ply**The local strains and local stress as in the 300 ply at the top surface are found using transformation equations as**D) Portion of load taken by each ply**Portion of load Nx taken by 00 ply = 4.464(104)(5)(10-3) = 223.2 N/m Portion of load Nx taken by 300 ply = 1.063(105)(5)(10-3) = 531.5 N/m Portion of load Nx taken by -450 ply = 4.903(104)(5)(10-3) = 245.2 N/m The sum total of the loads shared by each ply is 1000 N/m, (223.2 + 531.5 + 245.2) which is the applied load in the x-direction, Nx.**Percentage of load Nx taken by 00 ply**Percentage of load Nx taken by 300 ply Percentage of load Nx taken by -450 ply

More Related